THIN FILM GROWTH TECHNIQUES: IMPORTANCE
OF THIN FILMS
Vikram Dev (A) College, Jeypore, (India)
The effect of growth technique on thin film growth is of considerable significance, as films grown by two
different growth techniques using same precursor materials usually have different properties. This is attributed
to the fact that the properties of the grown films depends on a great extent on their structure, micro structure and
the type of impurities present. In addition, films grown using the same growth technique but variant process
parameters, show different properties due to the variation of the process parameters. Therefore, controlling the
process parameters is the key way to tailor the properties of the grown films. In this chapter, therefore, it is
important and necessary to make a detailed investigation on the techniques used for the deposition of thin films.
It is known that, the improved performance of the thin films in various fields of application is directly related to
their exposed surface-to-volume ratio and therefore films made using high surface area often exhibits
dramatically improved performance [1-2]. The majority of the nano-material was tested in thick film form
synthesized by screen-printing technique. Proper control of the grain size of these thick films remains one of the
major research issues. The thick film devices must be heated to sufficiently high temperature for film integrity
as well as grain-to-grain connectivity. At the same time the processing temperature should not be too high so
that rapid grain growth takes place with rapid decrease of the open porosity. Therefore, the material fabrication
process needs to be directed towards the thin film technology (with appropriate microstructure control) rather
than adopting the traditional thick film technology starting from powders. The stability of nano-crystalline thick
films also remains one of the major research issues. The stability problem can be partially circumvented by
fabricating thin film sensing materials.
The above advantages of thin films have boosted the growth of high quality thin films (ZnO thin film in the
present work). ZnO thin films can be grown by various techniques, such as: metal organic chemical vapor
deposition (MOCVD) , pulsed-laser deposition (PLD) , molecular beam epitaxy (MBE) , sputtering ,
chemical spray pyrolysis , screen printing , chemical solution deposition (CSD) technique , chemical
vapor deposition (CVD) , sol gel spin coating technique  and so on. Using some of these growth
techniques it is possible to control the thickness, micro structure and grain size of the films precisely.
Out of the above cited deposition techniques MOCVD is one of the most important techniques for proper
control of the deposition parameters. It is a vapor-phase deposition process in which organometallic precursors
are used. Despite of a number of factors that is to be optimized during the growth, following are the advantages
of MOCVD growth technique: (i) material can be grown at atmospheric pressure (ii) low growth temperature
can be achieved (iii) thickness and microstructure can be controlled precisely (iv) uniform deposition can be
done (v) high growth rate can be achieved, and so on . Viewing in light of the above description, in this
II. GROWTH OF ZNO THIN FILMS USING MOCVD
As ZnO is prone to form in various types of structures, growth of ultra thin ZnO film requires a suitable
technique where high deposition rate can be achieved. For high deposition rate the flow rate of zinc precursor
should be high and there should be appropriate oxygen flow rate. MOCVD is proved to be a promising method
for controlling this flow rate of the precursors, thus controlling the rate of deposition and hence the quality of
the films. Therefore, in this section the growth of ultra thin ZnO thin films using MOCVD technique is
described in details. It begins with the results of the MOCVD growth of ZnO that are already reported in the
literature. Next, the effects of various parameters such as substrate, temperature, and flow rate on the growth of
ZnO thin films are depicted. There follows the optimization of ZnO thin films.
2.1 History of Growth
In the past decades, good quality ZnO thin films have been grown using MOCVD technique by optimizing
different parameters. In 1980, Lau et al.  havegrown ZnO thin films on sapphire substrate using diethyl zinc
(DEZn) as zinc precursor, H2O, CO2, and N2O as oxygen precursor and H2 as carrier gas. They recorded a
maximum growth rate of 5.1µm/hr at 400oC in presence of DEZn and H2O, but explained that in order to retain
epitaxy the growth rates had to be kept low. They showed H2 to be a poor carrier gas for ZnO growth. In 1981
Roth and Williams  have grown ZnO thin films using DEZn and O2 on Pyrex glass substrates, by varying
the deposition rate and substrate temperature. They also encountered similar problems as Lau et al., as DEZn
and O2 react spontaneously even at room temperature, causing the deposition of white ZnO powder on the
reactor walls. They observed an increase in growth rate above 370oC, which reaches a maximum value of 2.4
mm/hr at 450oC. Wright et al.  in 1984 deposited ZnO thin films on GaP and glass slides using
oxygen-containing heterocycle compounds such as furan, tetrahydrofuran, and tetrahydropyran to avoid the premature
reactions observed with H2O and O2. They got promising results regarding the quality of the film, however the
growth rate decreased to 1.9 mm/hr which they thought may be due to the reaction between dimethyl zinc and
these heterocyclic compounds. Finally, these problems were overcome in 1985 when Oda et al.  used
alcohols like methanol (MeOH), ethanol (EtOH), or tert-butanol as oxygen precursors. By adjusting the flow of
carrier gas (He) through the bubblers, they set their DEZn and alcohol flow rates at 54 and 1300~9000
mmol/min, respectively, and studied the growth from 200 to 400oC. Of all the alcohols tested, they observed a
crystalline layer of ZnO and the highest degree of c-axis orientation, at lowest temperature (200oC) using tert
-butanol. They also reported that the n-type conductivity of the grown ZnO films was related to the presence of
donor levels resulting from oxygen vacancies. Then after thirteen years, in 1998, Hahn et al.  reported
MOCVD growth of ZnO using alcohol (tert-butanol) as the oxygen precursor. Keeping the horizontal reactor
chamber at atmospheric pressure, they varied the temperature from 260 to 410oC and the VI: II ratio between 2
and 18:1 during growth. They have noticed that the grown films become brownish at a substrate temperature of
360oC and at VI: II ratios less than 2:1 and reported that the oxygen deficiencies are responsible for the
brownish color of the films. They also observed the c-axis orientation of ZnO thin films with grain sizes
averaging 100 nm.
After that numbers of researches [17-18] were carried out focusing on various aspects such as cleanness of the
transparent electrodes, piezoelectric devices or SAW filters and specially at photonic devices. Eriksson et al.
 in 2009 have studied the oxygen gas sensitivity of electrochemically produced ZnO nanoparticles and PE–
MOCVD grown ZnO films.
2.2 Effect of Substrate on the Growth of ZnO thin Films
Though using MOCVD it is possible to grow very good quality of films but the quality of the film depends
strongly on the quality of the substrate. It is reported that a low lattice mismatch between the film and substrate
improves the film quality and large mismatch usually leads to structural defects and larger strain on the film
surface . As stated by G. Korotcenkov  selection of substrates with corresponding lattice parameter and
thermal expansion coefficient, can reduce the strain and at suitable conditions it is also possible to grow
epitaxial metal oxide thin films. Hence proper selection of the substrates is one of the key issues for the growth
of good quality thin films. For the growth of ZnO thin films a large number of substrates are available, such as
GaN, sapphire, fused quartz, Si, and so on. GaN is an ideal substrate for the growth of ZnO, being similar lattice
constants and having wurtzite structure. However, it does not have a native substrate. So first the buffer layers of
GaN are grown for the growth of ZnO . Sapphire (a = 4.75 Å, c = 12.99 Å) is also used largely for the
growth of ZnO thin films.
Besides this, the most important point that is taken into consideration while choosing a substrate is that for
certain characterization of the grown films certain substrates are needed; e.g. for Hall measurements of ZnO thin
films one needs a non-conducting substrate and for optical characterization a transparent substrate (like fused
silica) is needed. In our work we have used fused silica as the substrate for the growth of ZnO thin films.
2.3 Influence of Temperature on the Properties of ZnO thin Films
Out of all the parameters that affect the quality of the thin films, one of the most important is the growth
temperature. This growth temperature affects quite a bit on the properties of the grown thin films. To study the
influence of growth temperature on the quality of the film, we have grown a number of ZnO thin films in the
temperature range 400-500oC, keeping the other parameters constant. Each film is grown for one hour duration
keeping the flow rates of the diethyl zinc (DEZn) and tert-butanol at 20 and 60 sccm, respectively. The
influence of flow rate will be discussed in the next section. The structural and micro structural properties are
studied in terms of X-ray diffraction pattern and FESEM micrographs respectively . Fig. 1 (a-c) shows the
XRD pattern of the grown films in the said temperature range.
As demonstrated from the XRD pattern all the grown films are textured along (002) plane. However, the
intensity of the (002) oriented peak differs significantly. The XRD pattern of the sample grown at 400oC (Fig.1
(a)) shows a weak (002) peak. This lower intensity may be attributed to the low growth temperature. Now
increasing temperature from 400°C to 450°C, as shown in Fig.1 (b), leads a significant enhancement in the
intensity of (002) diffraction peaks. This shows the preferential orientation of the ZnO grains along (002)
planes. However, further increase in temperature reduces the preferential orientation in ZnO grains, as observed
from Fig. 1 (c). This may be due to the faster reaction rate at higher growth temperatures which hinders the
crystallization reaction .
Fig. 2 (a-c) shows the FESEM images of the grown ZnO thin films in the temperature range 400- 500oC.
Fig.2: FESEM images of the ZnO thin films grown at different temperatures, (a) 400oC, (b) 450oC, and (c) 500oC [Reproduced from Ref. 22].
As observed from the figure the microstructure of the grown samples depends strongly on the growth
temperatures. At 400°C (lowest growth temperature in the present study) the microstructure reveals presence of
individual grains separated by voids. No prominent grain boundaries are observed. This is attributed to the fact
that at lower growth temperatures the surface adatoms may not have sufficient mobility. Now with increasing
growth temperature, at 450°C, the surface morphology shows distinct grains separated by grain boundaries
without the presence of voids. However, with further increase in temperature the morphology becomes sparse,
which may be due to the sintering and grain growth at higher temperature. In view of the structural and micro
structural characterization of the samples, it appears that 450oC is the optimum temperature for the growth of
ZnO thin films.
2.4 Influence of Flow Rate on the Properties of ZnO thin Films
The VI: II ratio during growth is a measure of the O-to-Zn ratio in the gas phase during the film deposition
process, which has a significant effect on the properties of ZnO. A low VI: II ratio will create oxygen vacancies
in the crystal lattice, while a high VI: II ratio will cause an abundance of oxygen producing various defects in
the material. These defects in turn affect the properties of the material to a large extent [24-25]. Pagni et. al. 
studied the effect of flow rate on the structural and optical properties of the ZnO thin films. They found that
decreasing the VI: II ratio from 60:1 to 10:1 lead the (002) XRD peak position to shift to higher values, which is
due to the generation of oxygen vacancies in the crystal as less oxygen enters the reactor tube. They have also
reported the largest optical band gap (3.24 eV) and the lowest Urbach tail E0 parameter (254 meV) for the
sample deposited at a VI: II ratio of 18:1. They reported an increase in carrier concentration from 5.2 × 1017 to
9.4 × 1019 with a decrease of flow rate from 60:1 to 10:1, which is also due to the creation of oxygen vacancies
which they have high nucleation densities, irregular grains of different sizes, and increased surface roughness. In
our work we have kept a lower VI: II ratio (3:1) to enable the formation of oxygen vacancies in the ZnO thin
films, as presence of oxygen vacancies will promote the use of ZnO thin films in various fields like gas sensor.
The author gratefully acknowledged IIT Kharagpur for providing the experimental facility.
. N.S. Ramgir, Y.K. Hwang, S.H. Jhung, I.S. Mulla, and J.S. Chang, Effect of Pt concentration on the
physicochemical properties and CO sensing activity of mesostructured SnO2, Sensors and Actuators B,
114, 2006, 275-282.
. N. Yamazoe, G. Sakai and K. Shimanoe, Oxide semiconductor gas sensors, Catalysis Surveys from Asia,
7, 2007, 63-75.
. S. Pati,S. B. Majumder, and P. Banerji, MOCVD grown ZnO ultra thin film gas sensors: Influence of
microstructure,Sensors and Actuators A, 213, 2014, 52–58.
. S. Majumdar and P. Banerji, Growth and characterization of urea doped p-type ZnO thin film grown by
pulsed laser deposition, Advanced Materials Research, 67, 2009, 127-130.
. C.-Y.J. Lu, L. Chang, K. H. Ploog and M. M. C. Chou, Epitaxial growth of nonpolar ZnO on MgO (1 0 0)
substrate by molecular beam epitaxy, Journal of Crystal Growth, 378, 2013, 172-176.
. S. Elmas and S. Korkmaz, Deposition of Al doped ZnO thin films on the different substrates with radio
frequency magnetron sputtering, Journal of Non-Crystalline Solids, 359, 2013, 69–72.
. P. S. Shewale, G. L. Agawane, S. W. Shin, A. V. Moholkar, J. Y. Lee, J.H. Kim and M. D. Uplane,
Thickness dependent H2S sensing properties of nanocrystalline ZnO thin films derived by advanced spray
pyrolysis, Sensors and Actuators B, 177, 2013, 695–702.
. S. Akbar, P. Dutta and C. Lee High temperature ceramic gas sensors: A review, International Journal of
Applied Ceramic Technology, 3, 2006, 302-311.
. M. Wang, S. H. Hahn, E. J. Kim, J. S. Kim, S. Kim, C. Park and K.-K. Koo, Chemical solution deposition
of ZnO thin films with controlled crystallite orientation and intense ultraviolet emission, Thin Solid Films,
516, 2008, 8599–8603.
.D. Kim, I. Yun and H. Kim, Fabrication of rough Al doped ZnO films deposited by low pressure chemical
vapor deposition for high efficiency thin film solar cells, Current Applied Physics, 10, 2010, S459–S462.
.S. Pati, P. Banerjiand S. B. Majumder, Properties of indium doped nanocrystalline ZnO thin films and
their enhanced gas sensing performance, RSC Advance, 5, 2015, 61230-61238.
.C. K. Lau, S. K. Tiku and K. M. Lakin, Growth of epitaxial ZnO thin films by organometallic chemical
vapor deposition, Journal of Electrochemical Society, 127, 1980, 1843-1847.
.A.P. Roth and D.F. Williams, Semiconducting Zinc Oxide films prepared by organic chemical vapor
deposition from diethyl zinc, Journal of Electrochemical Society, 128, 1981, 2684-2686.
.P.J. Wright, R. J. M. Griffiths and B. Cockayne, The use of heterocyclic compound in the organometallic
.S. Oda, H. Tokunaga, N. Kitajima, J. -I. Hanna, I. Shimizu and H. Kokado, Highly oriented ZnO films
prepared by MOCVD from diethyl zinc and alcohols, Japanese Journal of Applied Physics, 24, 1985,
.B. Hahn, G. Heindel, E. Pschorr-Schoberer and W. Gebhardt, MOCVD layer growth of ZnO using DMZn
and butanol, Semiconductor Science and Technology, 13, 1998, 788-791.
.N. Oleynik, M. Adam, A. Krtschil, J. Blasing, A. Dadgar, F. Bertram, D. Forster, A. Diez, A. Greiling, M.
Seip, J. Christen and A. Krost, Metal organic chemical vapor phase deposition of ZnO with different
O-precursors, Journal of Crystal Growth, 248, 2003, 14–19.
.C. Kirchner, Th. Gruber, F. Reub, K. Thonke, A. Waag, Ch. Gieben and M. Heuken, MOVPE growth of
ZnO using various oxygen precursors, Journal of Crystal Growth, 248, 2003, 20-24.
.J. Eriksson, V. Khranovskyy, F. Soderlind, P.-O. Kall, R. Yakimova and A. L. Spetz, ZnO Nanoparticles
or ZnO films: A comparison of the gas sensing capabilities, Sensors and Actuators B, 137, 2009, 94–102.
.G. Korotcenkov, Gas response control through structural and chemical modiﬁcation of metal oxide films:
State of the art and approaches, Sensors and Actuators B, 107, 2005, 209–232.
.B. M. Ataev, W. V. Lundin, V. V. Mamedov, A. M. Bagamadova and E. E. Zavarin, Low-pressure
chemical vapor deposition growth of high-quality ZnO films on Epi-GaN/α-Al2O3, Journal of Physics
Condensed Matter, 13, 2001, L211–L214.
.S. Pati and P. Banerji, Effect of temperature on the structural and morphological characteristics of ZnO
thin films grown by MOCVD, International Journal of Computer & Mathematical Sciences, 3 (7), 2014,
.B. S. Li, Y. C. Liu, D. Z. Shen, J. Y. Zhang, Y. M. Lu and X. W. Fan, Effects of RF power on properties
of ZnO thin films grown on Si (0 0 1) substrate by plasma enhanced chemical vapor deposition, Journal of
Crystal Growth, 249, 2003, 179–185.
.O. D. Pagni, On the MOCVD growth of ZnO, Ph. D. Thesis, Faculty of Science at the University of Port
.S. Choopun, R. D. Vispute, W. Noch, A. Balsamo, R. P. Sharma, T. Venkatesan, A. Iliadis and D. C.
Look, Oxygen pressure-tuned epitaxy and optoelectronic properties of laser-deposited ZnO films on